#------------------------------------------------------------------------------
#$Date: 2020-07-04 04:34:08 +0300 (Sat, 04 Jul 2020) $
#$Revision: 253704 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/24/08/7240815.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7240815
loop_
_publ_author_name
'Zhang, Zaixiang'
'SUZUKI, Masahiro'
'YANG, Yu'
'Yoshikawa, Isao'
'Yin, Qiuxiang'
'Houjou, Hirohiko'
_publ_section_title
;
 Seed-triggered solid-to-solid transformation between color polymorphs:
 Striking differences between quasi-isomorphous crystals of
 dichloro-substituted salicylideneaniline regioisomers
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/D0CE00679C
_journal_year                    2020
_chemical_formula_moiety         'C13 H9 Cl2 N O'
_chemical_formula_sum            'C13 H9 Cl2 N O'
_chemical_formula_weight         266.11
_chemical_melting_point          427
_chemical_name_common
N-(2-Hydroxy-4-chlorobenzylidene)-4-chloroaniline
_chemical_name_systematic        N-(4?-chlorosalicylidene)-4-chloroaniline
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/1
_audit_update_record
;
2020-05-05 deposited with the CCDC.	2020-07-02 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 93.2393(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.004(6)
_cell_length_b                   4.688(3)
_cell_length_c                   11.919(7)
_cell_measurement_reflns_used    1817
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      27.50
_cell_measurement_theta_min      3.40
_cell_volume                     558.1(6)
_computing_cell_refinement       'CrystalClear-SM Expert 2.0 r3'
_computing_data_collection
'CrystalClear-SM Expert 2.0 r3 (Rigaku, 2009)'
_computing_data_reduction        'CrystalClear-SM Expert 2.0 r3'
_computing_molecular_graphics    'CrystalStructure 4.2.4'
_computing_publication_material  'CrystalStructure 4.2.4 (Rigaku, 2016)'
_computing_structure_refinement  'SHELXL-2018/1 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXS Version 2013/1 (Sheldrick, 2008)'
_diffrn_ambient_temperature      93(2)
_diffrn_detector_area_resol_mean 7.111
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'VariMax DW with Saturn'
_diffrn_measurement_method       ω
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0530
_diffrn_reflns_av_unetI/netI     0.0462
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            6122
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.491
_diffrn_reflns_theta_min         2.039
_exptl_absorpt_coefficient_mu    0.560
_exptl_absorpt_correction_T_max  0.975
_exptl_absorpt_correction_T_min  0.862
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'REQAB (Rigaku, 1998)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    1.584
_exptl_crystal_description       plate
_exptl_crystal_F_000             272
_exptl_crystal_recrystallization_method
'Re-crystallisation from solvent: acetone'
_exptl_crystal_size_max          0.190
_exptl_crystal_size_mid          0.180
_exptl_crystal_size_min          0.080
_refine_diff_density_max         0.406
_refine_diff_density_min         -0.406
_refine_diff_density_rms         0.085
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.265
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     81
_refine_ls_number_reflns         1275
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.265
_refine_ls_R_factor_all          0.0576
_refine_ls_R_factor_gt           0.0504
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+1.5632P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1187
_refine_ls_wR_factor_ref         0.1208
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1133
_reflns_number_total             1275
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0ce00679c3.cif
_cod_data_source_block           4CC-o
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               7240815
_shelx_shelxl_version_number     2018/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.901
_shelx_estimated_absorpt_t_max   0.957
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.4590(5) 0.2602(10) 0.3052(4) 0.0196(10) Uani 0.5 1 d . . P A -1
H1 H 0.496645 0.119548 0.337138 0.029 Uiso 0.5 1 calc R U P A -1
C1 C 0.3694(3) 0.3652(6) 0.3698(3) 0.0137(6) Uani 1 1 d . . . . .
H2 H 0.434210 0.289047 0.322906 0.016 Uiso 0.5 1 calc R U P A 2
C2 C 0.2784(3) 0.5684(7) 0.3273(3) 0.0146(6) Uani 1 1 d . . . . .
H3 H 0.281221 0.632022 0.251760 0.018 Uiso 1 1 calc R U . . .
C3 C 0.1840(3) 0.6765(7) 0.3963(3) 0.0141(6) Uani 1 1 d . . . . .
C4 C 0.1781(3) 0.5903(7) 0.5077(3) 0.0180(7) Uani 1 1 d . . . . .
H4 H 0.113159 0.668040 0.554225 0.022 Uiso 1 1 calc R U . . .
C5 C 0.2695(3) 0.3877(7) 0.5491(3) 0.0178(7) Uani 1 1 d . . . . .
H5 H 0.266618 0.326302 0.624918 0.021 Uiso 1 1 calc R U . . .
C6 C 0.3659(3) 0.2722(6) 0.4814(3) 0.0126(6) Uani 1 1 d . . . . .
Cl1 Cl 0.07060(7) 0.92695(16) 0.34058(7) 0.0184(2) Uani 1 1 d . . . . .
C7 C 0.4601(17) 0.053(4) 0.5257(14) 0.0132(8) Uiso 0.5 1 d . . P B -1
H6 H 0.456776 -0.000669 0.602399 0.016 Uiso 0.5 1 calc R U P B -1
N1 N 0.5452(15) -0.068(3) 0.4671(11) 0.0132(8) Uiso 0.5 1 d . . P B -1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C1 O1 H1 109.5 . . ?
O1 C1 C2 119.8(3) . . ?
O1 C1 C6 119.7(3) . . ?
C2 C1 C6 120.5(3) . . ?
C2 C1 H2 119.7 . . ?
C6 C1 H2 119.7 . . ?
C3 C2 C1 119.2(3) . . ?
C3 C2 H3 120.4 . . ?
C1 C2 H3 120.4 . . ?
C2 C3 C4 121.9(3) . . ?
C2 C3 Cl1 118.2(2) . . ?
C4 C3 Cl1 119.9(2) . . ?
C5 C4 C3 118.3(3) . . ?
C5 C4 H4 120.8 . . ?
C3 C4 H4 120.8 . . ?
C4 C5 C6 121.3(3) . . ?
C4 C5 H5 119.3 . . ?
C6 C5 H5 119.3 . . ?
C5 C6 C1 118.8(3) . . ?
C5 C6 C7 120.7(7) . . ?
C1 C6 C7 120.5(7) . . ?
N1 C7 C6 123.5(8) . . ?
N1 C7 H6 118.2 . . ?
C6 C7 H6 118.2 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 C1 1.310(5) . ?
O1 H1 0.8400 . ?
C1 C2 1.393(4) . ?
C1 C6 1.402(4) . ?
C1 H2 0.9500 . ?
C2 C3 1.383(4) . ?
C2 H3 0.9500 . ?
C3 C4 1.392(4) . ?
C3 Cl1 1.738(3) . ?
C4 C5 1.390(4) . ?
C4 H4 0.9500 . ?
C5 C6 1.401(4) . ?
C5 H5 0.9500 . ?
C6 C7 1.472(17) . ?
C7 N1 1.266(6) . ?
C7 H6 0.9500 . ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O1^a H1^a N1^a 0.84 1.82 2.579(15) 148.8 . yes
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 C1 C2 C3 179.7(4) . . . . ?
C6 C1 C2 C3 -0.4(5) . . . . ?
C1 C2 C3 C4 0.7(5) . . . . ?
C1 C2 C3 Cl1 -179.3(2) . . . . ?
C2 C3 C4 C5 -0.6(5) . . . . ?
Cl1 C3 C4 C5 179.4(2) . . . . ?
C3 C4 C5 C6 0.2(5) . . . . ?
C4 C5 C6 C1 0.2(5) . . . . ?
C4 C5 C6 C7 -178.5(8) . . . . ?
O1 C1 C6 C5 179.8(4) . . . . ?
C2 C1 C6 C5 -0.1(4) . . . . ?
O1 C1 C6 C7 -1.4(9) . . . . ?
C2 C1 C6 C7 178.6(8) . . . . ?
C5 C6 C7 N1 176.7(4) . . . . ?
C1 C6 C7 N1 -2.0(11) . . . . ?
